#------------------------------------------------------------------------------
#$Date: 2019-09-13 09:51:30 +0300 (Fri, 13 Sep 2019) $
#$Revision: 218251 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/38/7233821.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7233821
loop_
_publ_author_name
'Hao Miao'
'Hong-Xiang Wan'
'Ming Liu'
'Yu Zhang'
'Xiao Xu'
'Wei-Wei Ju'
'Dun-ru Zhu'
'Yan Xu'
_publ_section_title
;
 Two novel organic-inorganic hybrid molybdenum(v) cobalt/nickel phosphate
 compounds based on isolated nanosized Mo/Co(Ni)/P cluster wheels
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              6554
_journal_page_last               6560
_journal_paper_doi               10.1039/C4TC00944D
_journal_volume                  2
_journal_year                    2014
_chemical_formula_sum            'C76 H127 Co17 Mo16 N18 O132 P24'
_chemical_formula_weight         6685.09
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 126.7600(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   29.724(4)
_cell_length_b                   24.623(3)
_cell_length_c                   20.687(3)
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      22.45
_cell_measurement_theta_min      2.22
_cell_volume                     12130(3)
_computing_cell_refinement       'SAINT (Bruker, 2005)'
_computing_data_collection       'APEX2 (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker Apex2 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0621
_diffrn_reflns_av_sigmaI/netI    0.0622
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            43123
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         1.23
_exptl_absorpt_coefficient_mu    2.170
_exptl_absorpt_correction_T_max  0.7807
_exptl_absorpt_correction_T_min  0.7228
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.830
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             6512
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.12
_refine_diff_density_max         3.984
_refine_diff_density_min         -2.180
_refine_diff_density_rms         0.241
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.046
_refine_ls_hydrogen_treatment    'riding model'
_refine_ls_matrix_type           full
_refine_ls_number_parameters     786
_refine_ls_number_reflns         10963
_refine_ls_number_restraints     340
_refine_ls_restrained_S_all      1.067
_refine_ls_R_factor_all          0.1100
_refine_ls_R_factor_gt           0.0695
_refine_ls_shift/su_max          0.038
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1611P)²+4.3103P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2152
_refine_ls_wR_factor_ref         0.2403
_reflns_number_gt                7250
_reflns_number_total             10963
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            1000001.cif
_cod_data_source_block           PCOD1000001
_cod_original_cell_volume        12130(2)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               7233821
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 1.077611(17) 0.36901(2) 0.85961(2) 0.03546(13) Uani 1 1 d . A .
Mo2 Mo 1.179144(17) 0.36955(2) 1.24321(2) 0.03581(13) Uani 1 1 d . A .
Mo3 Mo 1.117346(17) 0.41072(2) 0.78767(2) 0.03857(13) Uani 1 1 d . A .
Mo4 Mo 1.271922(18) 0.41045(2) 1.36897(2) 0.03936(14) Uani 1 1 d . A .
Co1 Co 0.5000 0.0000 0.0000 0.0643(6) Uani 1 4 d SD . .
Co2 Co 0.96541(3) 0.43276(3) 0.65879(4) 0.0419(2) Uani 1 1 d . . .
Co3 Co 1.26999(3) 0.43181(3) 1.19224(4) 0.0414(2) Uani 1 1 d . A .
Co4 Co 1.16018(3) 0.43187(3) 1.39130(4) 0.0436(2) Uani 1 1 d . . .
Co5 Co 1.22140(3) 0.43085(4) 1.00476(4) 0.0430(2) Uani 1 1 d . A .
P1 P 1.05026(8) 0.5000 0.63809(10) 0.0427(6) Uani 1 2 d SD . .
P2 P 1.22191(8) 0.5000 0.87087(11) 0.0473(6) Uani 1 2 d SD . .
P3 P 1.27770(9) 0.5000 1.49460(11) 0.0476(7) Uani 1 2 d S . .
P4 P 0.86683(9) 0.5000 0.50679(11) 0.0560(7) Uani 1 2 d SD . .
P5 P 1.35108(8) 0.5000 1.35809(12) 0.0463(7) Uani 1 2 d SD . .
P6 P 1.33075(8) 0.5000 1.13334(13) 0.0526(7) Uani 1 2 d S . .
P7 P 1.16011(9) 0.35115(10) 1.06542(13) 0.0247(6) Uani 0.50 1 d P A 1
P7A P 1.14786(14) 0.37828(19) 1.05907(18) 0.0645(12) Uani 0.50 1 d P A 2
P8 P 1.06264(9) 0.35196(10) 1.23729(12) 0.0251(6) Uani 0.50 1 d P . 1
P8A P 1.05773(12) 0.38204(17) 1.21837(17) 0.0546(10) Uani 0.50 1 d P . 2
P9 P 1.16247(12) 0.5000 1.25919(16) 0.0278(9) Uani 0.50 2 d SPD . 1
P9A P 1.18804(13) 0.5000 1.21586(17) 0.0415(12) Uani 0.50 2 d SPD . 2
P10A P 1.10456(12) 0.5000 0.90210(15) 0.0332(10) Uani 0.50 2 d SPD . 1
P10 P 1.04779(11) 0.5000 0.82521(16) 0.0360(10) Uani 0.50 2 d SPD . 2
O1 O 1.04074(13) 0.40068(15) 0.75175(18) 0.0374(10) Uani 1 1 d . . .
O2 O 1.15188(13) 0.39898(16) 0.90182(18) 0.0398(10) Uani 1 1 d . . .
O3 O 0.99826(14) 0.35814(19) 0.8322(2) 0.0542(13) Uani 1 1 d . . .
O4 O 1.24552(13) 0.40071(15) 1.25802(18) 0.0390(10) Uani 1 1 d . . .
O5 O 1.19859(13) 0.39964(16) 1.34504(18) 0.0406(11) Uani 1 1 d . . .
O6 O 1.29551(15) 0.44872(18) 1.47222(19) 0.0512(13) Uani 1 1 d . . .
O7 O 1.34093(14) 0.44802(17) 1.3899(2) 0.0467(12) Uani 1 1 d . . .
O8 O 1.09987(15) 0.5000 0.8214(2) 0.0553(16) Uani 1 2 d SD . .
O9 O 1.14479(15) 0.3589(2) 1.1213(2) 0.0593(14) Uani 1 1 d . . .
O10 O 1.19055(14) 0.44862(18) 0.82368(19) 0.0508(12) Uani 1 1 d . . .
O11 O 1.08375(14) 0.44891(17) 0.67928(19) 0.0499(11) Uani 1 1 d U . .
O12 O 1.10708(14) 0.35614(19) 0.97900(19) 0.0524(13) Uani 1 1 d . . .
O13 O 1.08128(13) 0.39249(17) 1.30713(19) 0.0440(11) Uani 1 1 d . . .
O14 O 1.29472(14) 0.44899(17) 1.11969(19) 0.0466(11) Uani 1 1 d . . .
O15 O 1.09770(14) 0.35815(19) 1.20711(19) 0.0538(12) Uani 1 1 d . . .
O16 O 1.06420(13) 0.45154(14) 0.88653(18) 0.0509(11) Uani 1 1 d D . .
O17 O 1.3163(2) 0.5000 1.2668(3) 0.0472(16) Uani 1 2 d S . .
O18 O 1.30500(16) 0.35215(19) 1.4134(2) 0.0581(15) Uani 1 1 d . . .
O19 O 1.20589(13) 0.39103(17) 1.08217(18) 0.0423(11) Uani 1 1 d . . .
O20 O 1.08374(14) 0.30291(16) 0.8437(2) 0.0509(12) Uani 1 1 d . . .
O21 O 1.2291(2) 0.5000 1.3120(2) 0.053(2) Uani 1 2 d SD . .
O22 O 1.14619(14) 0.45086(15) 1.1998(2) 0.0499(13) Uani 1 1 d D . .
O23 O 1.2161(2) 0.5000 1.4579(3) 0.0487(17) Uani 1 2 d S . .
O24 O 0.9942(2) 0.5000 0.6257(3) 0.0512(17) Uani 1 2 d SU . .
O25 O 1.13129(15) 0.35264(17) 0.7602(2) 0.0526(12) Uani 1 1 d . . .
O26 O 1.19523(16) 0.30347(17) 1.2634(2) 0.0575(14) Uani 1 1 d . . .
O27 O 1.2358(2) 0.5000 0.9555(3) 0.0557(17) Uani 1 2 d S . .
O28 O 1.1296(2) 0.5000 1.3025(3) 0.060(2) Uani 1 2 d SD . .
O29 O 0.88203(15) 0.44998(19) 0.5598(2) 0.0591(13) Uani 1 1 d . . .
O30 O 1.20833(19) 0.5000 1.1579(3) 0.079(3) Uani 1 2 d SD . .
O31 O 0.9837(2) 0.5000 0.7450(3) 0.073(2) Uani 1 2 d SD . .
O32 O 1.1643(2) 0.5000 0.9893(3) 0.085(2) Uani 1 2 d SD . .
O33 O 1.3854(3) 0.5000 1.2067(6) 0.121(4) Uani 1 2 d S . .
O35 O 0.8108(5) 0.5000 0.4278(6) 0.075(4) Uani 0.50 2 d SPDU B 1
O35A O 0.8847(4) 0.5000 0.4535(5) 0.071(3) Uani 0.50 2 d SPDU B 2
O36 O 1.3085(5) 0.5000 1.5849(6) 0.157(6) Uani 1 2 d S . .
O37 O 1.2746(3) 0.5000 0.8775(6) 0.187(4) Uani 1 2 d SDU . .
O38 O 1.4131(4) 0.5000 1.3919(8) 0.200(5) Uani 1 2 d SDU . .
N1 N 0.9590(2) 0.3702(2) 0.5824(2) 0.0607(17) Uani 1 1 d . . .
N2 N 1.3286(2) 0.3670(2) 1.2393(3) 0.0581(17) Uani 1 1 d . . .
N3 N 1.1979(3) 0.3701(2) 1.4793(3) 0.0873(18) Uani 1 1 d DU . .
N1A N 1.27094(5) 0.36953(3) 1.00087(4) 0.0941(16) Uani 1 1 d DU . .
C1A C 1.26581(8) 0.31543(7) 1.0053(3) 0.118(3) Uani 0.50 1 d PDU A 1
H1AA H 1.2342 0.2978 0.9943 0.142 Uiso 0.50 1 calc PR A 1
C2A C 1.31408(7) 0.29111(13) 1.0283(2) 0.126(2) Uani 0.50 1 d PDU A 1
C3A C 1.32554(8) 0.3754(4) 1.0316(4) 0.115(3) Uani 0.50 1 d PDU A 1
H3AA H 1.3456 0.4076 1.0533 0.138 Uiso 0.50 1 calc PR A 1
N2A N 1.34999(13) 0.3237(2) 1.0264(4) 0.124(3) Uani 0.50 1 d PDU A 1
C2B C 1.35821(3) 0.30982(5) 1.07723(5) 0.131(3) Uani 0.50 1 d PDU A 2
C5B C 1.25091(5) 0.33415(3) 0.93803(6) 0.125(3) Uani 0.50 1 d PDU A 2
H5BA H 1.2183 0.3437 0.8881 0.150 Uiso 0.50 1 calc PR A 2
C4B C 1.27569(3) 0.28567(4) 0.94376(14) 0.128(3) Uani 0.50 1 d PDU A 2
H4BA H 1.2558 0.2569 0.9087 0.153 Uiso 0.50 1 calc PR A 2
C3B C 1.33205(4) 0.28298(7) 1.00515(6) 0.123(3) Uani 0.50 1 d PDU A 2
H3BA H 1.3541 0.2614 0.9973 0.147 Uiso 0.50 1 calc PR A 2
C1B C 1.31401(3) 0.33929(5) 1.06306(8) 0.120(2) Uani 0.50 1 d PDU A 2
H1BA H 1.3130 0.3386 1.1071 0.144 Uiso 0.50 1 calc PR A 2
C1 C 0.9682(3) 0.3186(3) 0.6076(4) 0.070(2) Uani 1 1 d . A .
H1A H 0.9844 0.3116 0.6616 0.084 Uiso 1 1 calc R . .
C2 C 0.9547(3) 0.2749(4) 0.5563(4) 0.095(3) Uani 1 1 d . . .
H2A H 0.9596 0.2392 0.5740 0.114 Uiso 1 1 calc R A .
C3 C 0.9332(3) 0.2874(4) 0.4769(4) 0.095(3) Uani 1 1 d . A .
H3A H 0.9246 0.2595 0.4408 0.114 Uiso 1 1 calc R . .
C4 C 0.9255(3) 0.3358(4) 0.4536(4) 0.096(3) Uani 1 1 d . . .
H4A H 0.9112 0.3434 0.4005 0.115 Uiso 1 1 calc R A .
C5 C 0.9376(3) 0.3763(4) 0.5043(3) 0.080(3) Uani 1 1 d . A .
H5A H 0.9307 0.4115 0.4842 0.096 Uiso 1 1 calc R . .
C6 C 1.3139(3) 0.3167(3) 1.2427(5) 0.081(3) Uani 1 1 d . A .
H6A H 1.2789 0.3122 1.2318 0.098 Uiso 1 1 calc R . .
C7 C 1.3451(3) 0.2718(4) 1.2604(5) 0.104(4) Uani 1 1 d . . .
H7A H 1.3321 0.2376 1.2612 0.125 Uiso 1 1 calc R A .
C8 C 1.3944(4) 0.2781(4) 1.2764(5) 0.101(3) Uani 1 1 d . A .
H8A H 1.4165 0.2476 1.2884 0.122 Uiso 1 1 calc R . .
C9 C 1.4139(3) 0.3258(4) 1.2763(5) 0.104(3) Uani 1 1 d U . .
H9A H 1.4490 0.3294 1.2873 0.125 Uiso 1 1 calc R A .
C10 C 1.3784(4) 0.3732(5) 1.2583(6) 0.123(4) Uani 1 1 d U A .
H10A H 1.3917 0.4078 1.2605 0.148 Uiso 1 1 calc R . .
C11 C 1.2165(5) 0.3786(4) 1.5540(4) 0.153(4) Uani 1 1 d DU A .
H11A H 1.2171 0.4136 1.5714 0.183 Uiso 1 1 calc R . .
C12 C 1.2352(5) 0.3352(3) 1.6070(6) 0.167(4) Uani 1 1 d DU . .
H12A H 1.2512 0.3423 1.6609 0.200 Uiso 1 1 calc R A .
C13 C 1.2310(5) 0.2829(4) 1.5835(5) 0.161(4) Uani 1 1 d DU A .
H13A H 1.2506 0.2549 1.6203 0.193 Uiso 1 1 calc R . .
C14 C 1.1978(5) 0.2745(4) 1.5058(5) 0.155(4) Uani 1 1 d DU . .
H14A H 1.1825 0.2405 1.4841 0.186 Uiso 1 1 calc R A .
C15 C 1.1869(5) 0.3182(3) 1.4587(5) 0.139(3) Uani 1 1 d DU A .
H15A H 1.1693 0.3107 1.4044 0.167 Uiso 1 1 calc R . .
O1W O 0.5175(14) -0.1805(15) 0.016(3) 0.169(6) Uani 0.25 1 d PU . .
O2W O 0.4283(2) -0.0339(5) -0.0299(6) 0.127(3) Uani 0.50 1 d PDU . .
O4W O 0.2270(3) 0.0000 0.3528(5) 0.120(3) Uani 1 2 d SU . .
O5W O 0.5000 -0.1725(15) 0.0000 0.184(6) Uani 0.50 2 d SPU . .
O5WA O 0.5000 -0.2251(14) 0.0000 0.193(4) Uani 0.50 2 d SPU . .
O3W O 0.2961(10) 0.0617(14) 0.2990(15) 0.129(5) Uani 0.25 1 d PU . .
O39 O 1.0361(4) 0.5000 0.5559(4) 0.136(3) Uani 1 2 d SDU . .
O2WA O 0.5267(4) -0.0309(5) 0.1084(4) 0.125(3) Uani 0.50 1 d PDU . 1
O2WB O 0.4727(4) -0.0682(3) 0.0183(7) 0.144(3) Uani 0.50 1 d PDU . 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O20 Mo1 O1 102.25(17) . .
O20 Mo1 O2 102.95(18) . .
O1 Mo1 O2 94.03(14) . .
O20 Mo1 O3 93.4(2) . .
O1 Mo1 O3 88.31(15) . .
O2 Mo1 O3 162.54(18) . .
O20 Mo1 O12 93.82(19) . .
O1 Mo1 O12 162.85(17) . .
O2 Mo1 O12 88.11(15) . .
O3 Mo1 O12 84.74(15) . .
O20 Mo1 O16 172.90(19) . .
O1 Mo1 O16 81.89(14) . .
O2 Mo1 O16 82.34(15) . .
O3 Mo1 O16 80.87(16) . .
O12 Mo1 O16 81.53(16) . .
O20 Mo1 Mo3 97.44(16) . .
O1 Mo1 Mo3 47.89(11) . .
O2 Mo1 Mo3 48.17(10) . .
O3 Mo1 Mo3 136.15(11) . .
O12 Mo1 Mo3 136.25(11) . .
O16 Mo1 Mo3 89.61(10) . .
O26 Mo2 O4 103.3(2) . .
O26 Mo2 O5 104.01(19) . .
O4 Mo2 O5 93.56(15) . .
O26 Mo2 O15 93.2(2) . .
O4 Mo2 O15 162.44(16) . .
O5 Mo2 O15 88.18(15) . .
O26 Mo2 O9 92.2(2) . .
O4 Mo2 O9 87.54(16) . .
O5 Mo2 O9 162.96(17) . .
O15 Mo2 O9 85.80(16) . .
O26 Mo2 O22 171.06(14) . .
O4 Mo2 O22 82.34(15) . .
O5 Mo2 O22 82.32(15) . .
O15 Mo2 O22 80.57(16) . .
O9 Mo2 O22 80.98(17) . .
O26 Mo2 Mo4 98.79(12) . .
O4 Mo2 Mo4 47.87(10) . .
O5 Mo2 Mo4 47.79(11) . .
O15 Mo2 Mo4 135.92(11) . .
O9 Mo2 Mo4 135.39(13) . .
O22 Mo2 Mo4 90.14(8) . .
O25 Mo3 O1 103.44(17) . .
O25 Mo3 O2 103.05(17) . .
O1 Mo3 O2 95.23(15) . .
O25 Mo3 O10 95.00(19) . .
O1 Mo3 O10 160.27(16) . .
O2 Mo3 O10 87.28(15) . .
O25 Mo3 O11 94.43(18) . .
O1 Mo3 O11 87.02(15) . .
O2 Mo3 O11 161.29(16) . .
O10 Mo3 O11 84.58(15) . .
O25 Mo3 O8 174.72(19) . .
O1 Mo3 O8 79.85(14) . .
O2 Mo3 O8 80.59(14) . .
O10 Mo3 O8 81.27(15) . .
O11 Mo3 O8 81.54(15) . .
O25 Mo3 Mo1 98.40(16) . .
O1 Mo3 Mo1 48.62(10) . .
O2 Mo3 Mo1 48.68(11) . .
O10 Mo3 Mo1 135.79(10) . .
O11 Mo3 Mo1 135.54(11) . .
O8 Mo3 Mo1 86.87(10) . .
O18 Mo4 O5 102.9(2) . .
O18 Mo4 O4 103.42(19) . .
O5 Mo4 O4 94.80(15) . .
O18 Mo4 O6 95.79(19) . .
O5 Mo4 O6 87.72(16) . .
O4 Mo4 O6 159.50(17) . .
O18 Mo4 O7 94.97(19) . .
O5 Mo4 O7 160.98(17) . .
O4 Mo4 O7 87.16(16) . .
O6 Mo4 O7 84.09(17) . .
O18 Mo4 O21 175.79(16) . .
O5 Mo4 O21 79.71(18) . .
O4 Mo4 O21 79.49(16) . .
O6 Mo4 O21 80.96(15) . .
O7 Mo4 O21 82.06(17) . .
O18 Mo4 Mo2 98.04(13) . .
O5 Mo4 Mo2 48.52(10) . .
O4 Mo4 Mo2 48.42(11) . .
O6 Mo4 Mo2 136.02(12) . .
O7 Mo4 Mo2 135.48(11) . .
O21 Mo4 Mo2 86.17(8) . .
O2WB Co1 O2WB 65.6(7) . 2_655
O2WB Co1 O2WB 114.4(7) . 6
O2WB Co1 O2WB 180.0(5) 2_655 6
O2WB Co1 O2WB 180.0(7) . 5_655
O2WB Co1 O2WB 114.4(7) 2_655 5_655
O2WB Co1 O2WB 65.6(7) 6 5_655
O2WB Co1 O2W 40.0(4) . .
O2WB Co1 O2W 94.0(5) 2_655 .
O2WB Co1 O2W 86.0(5) 6 .
O2WB Co1 O2W 140.0(4) 5_655 .
O2WB Co1 O2W 86.0(5) . 6
O2WB Co1 O2W 140.0(4) 2_655 6
O2WB Co1 O2W 40.0(4) 6 6
O2WB Co1 O2W 94.0(5) 5_655 6
O2W Co1 O2W 49.0(7) . 6
O2WB Co1 O2W 140.0(4) . 5_655
O2WB Co1 O2W 86.0(5) 2_655 5_655
O2WB Co1 O2W 94.0(5) 6 5_655
O2WB Co1 O2W 40.0(4) 5_655 5_655
O2W Co1 O2W 180.0(8) . 5_655
O2W Co1 O2W 131.0(7) 6 5_655
O2WB Co1 O2W 94.0(5) . 2_655
O2WB Co1 O2W 40.0(4) 2_655 2_655
O2WB Co1 O2W 140.0(4) 6 2_655
O2WB Co1 O2W 86.0(5) 5_655 2_655
O2W Co1 O2W 131.0(7) . 2_655
O2W Co1 O2W 180.0(6) 6 2_655
O2W Co1 O2W 49.0(7) 5_655 2_655
O2WB Co1 O2WA 92.3(5) . 6
O2WB Co1 O2WA 126.2(4) 2_655 6
O2WB Co1 O2WA 53.8(4) 6 6
O2WB Co1 O2WA 87.7(5) 5_655 6
O2W Co1 O2WA 97.9(5) . 6
O2W Co1 O2WA 80.0(4) 6 6
O2W Co1 O2WA 82.1(5) 5_655 6
O2W Co1 O2WA 100.0(4) 2_655 6
O2WB Co1 O2WA 53.8(4) . .
O2WB Co1 O2WA 87.7(5) 2_655 .
O2WB Co1 O2WA 92.3(5) 6 .
O2WB Co1 O2WA 126.2(4) 5_655 .
O2W Co1 O2WA 80.0(4) . .
O2W Co1 O2WA 97.9(5) 6 .
O2W Co1 O2WA 100.0(4) 5_655 .
O2W Co1 O2WA 82.1(5) 2_655 .
O2WA Co1 O2WA 44.1(7) 6 .
O2WB Co1 O2WA 87.7(5) . 2_655
O2WB Co1 O2WA 53.8(4) 2_655 2_655
O2WB Co1 O2WA 126.2(4) 6 2_655
O2WB Co1 O2WA 92.3(5) 5_655 2_655
O2W Co1 O2WA 82.1(5) . 2_655
O2W Co1 O2WA 100.0(4) 6 2_655
O2W Co1 O2WA 97.9(5) 5_655 2_655
O2W Co1 O2WA 80.0(4) 2_655 2_655
O2WA Co1 O2WA 180.000(1) 6 2_655
O2WA Co1 O2WA 135.9(7) . 2_655
O2WB Co1 O2WA 126.2(4) . 5_655
O2WB Co1 O2WA 92.3(5) 2_655 5_655
O2WB Co1 O2WA 87.7(5) 6 5_655
O2WB Co1 O2WA 53.8(4) 5_655 5_655
O2W Co1 O2WA 100.0(4) . 5_655
O2W Co1 O2WA 82.1(5) 6 5_655
O2W Co1 O2WA 80.0(4) 5_655 5_655
O2W Co1 O2WA 97.9(5) 2_655 5_655
O2WA Co1 O2WA 135.9(7) 6 5_655
O2WA Co1 O2WA 180.0(8) . 5_655
O2WA Co1 O2WA 44.1(7) 2_655 5_655
O1 Co2 O29 168.70(17) . .
O1 Co2 N1 88.84(16) . .
O29 Co2 N1 83.90(18) . .
O1 Co2 O13 94.14(14) . 2_757
O29 Co2 O13 78.22(15) . 2_757
N1 Co2 O13 96.9(2) . 2_757
O1 Co2 O24 100.13(16) . .
O29 Co2 O24 89.80(18) . .
N1 Co2 O24 101.3(2) . .
O13 Co2 O24 156.94(18) 2_757 .
O1 Co2 O31 85.96(14) . .
O29 Co2 O31 102.01(17) . .
N1 Co2 O31 172.6(2) . .
O13 Co2 O31 88.68(19) 2_757 .
O24 Co2 O31 74.5(2) . .
O4 Co3 O14 169.65(17) . .
O4 Co3 N2 86.2(2) . .
O14 Co3 N2 86.3(2) . .
O4 Co3 O17 98.45(19) . .
O14 Co3 O17 90.4(2) . .
N2 Co3 O17 105.23(17) . .
O4 Co3 O19 95.02(15) . .
O14 Co3 O19 78.58(15) . .
N2 Co3 O19 95.65(17) . .
O17 Co3 O19 155.77(14) . .
O4 Co3 O30 86.72(18) . .
O14 Co3 O30 101.12(19) . .
N2 Co3 O30 172.0(2) . .
O17 Co3 O30 72.20(15) . .
O19 Co3 O30 88.64(15) . .
O5 Co4 O29 169.48(18) . 2_757
O5 Co4 N3 88.1(2) . .
O29 Co4 N3 84.2(2) 2_757 .
O5 Co4 O13 95.19(15) . .
O29 Co4 O13 78.84(16) 2_757 .
N3 Co4 O13 97.7(2) . .
O5 Co4 O23 99.6(2) . .
O29 Co4 O23 88.9(2) 2_757 .
N3 Co4 O23 101.51(18) . .
O13 Co4 O23 156.05(15) . .
O5 Co4 O28 88.43(19) . .
O29 Co4 O28 99.9(2) 2_757 .
N3 Co4 O28 173.7(3) . .
O13 Co4 O28 87.87(15) . .
O23 Co4 O28 73.93(14) . .
O2 Co5 O14 169.19(17) . .
O2 Co5 N1A 88.81(12) . .
O14 Co5 N1A 85.49(12) . .
O2 Co5 O19 93.86(15) . .
O14 Co5 O19 78.06(15) . .
N1A Co5 O19 99.49(12) . .
O2 Co5 O27 100.04(16) . .
O14 Co5 O27 90.13(17) . .
N1A Co5 O27 101.77(15) . .
O19 Co5 O27 154.74(18) . .
O2 Co5 O32 86.40(15) . .
O14 Co5 O32 100.40(17) . .
N1A Co5 O32 171.08(18) . .
O19 Co5 O32 88.3(2) . .
O27 Co5 O32 71.7(2) . .
O39 P1 O11 106.5(3) . 6_565
O39 P1 O11 106.5(3) . .
O11 P1 O11 112.7(3) 6_565 .
O39 P1 O24 105.9(5) . .
O11 P1 O24 112.3(2) 6_565 .
O11 P1 O24 112.3(2) . .
O37 P2 O10 105.4(3) . .
O37 P2 O10 105.4(3) . 6_565
O10 P2 O10 111.8(3) . 6_565
O37 P2 O27 110.1(5) . .
O10 P2 O27 111.9(2) . .
O10 P2 O27 111.9(2) 6_565 .
O23 P3 O36 106.1(6) . .
O23 P3 O6 112.39(19) . .
O36 P3 O6 108.0(3) . .
O23 P3 O6 112.39(19) . 6_565
O36 P3 O6 108.0(3) . 6_565
O6 P3 O6 109.8(4) . 6_565
O35 P4 O35A 81.1(7) . .
O35 P4 O29 116.6(3) . .
O35A P4 O29 116.8(3) . .
O35 P4 O29 116.6(3) . 6_565
O35A P4 O29 116.8(3) . 6_565
O29 P4 O29 107.6(3) . 6_565
O17 P5 O38 107.8(6) . .
O17 P5 O7 111.59(17) . 6_565
O38 P5 O7 107.1(3) . 6_565
O17 P5 O7 111.59(18) . .
O38 P5 O7 107.1(3) . .
O7 P5 O7 111.5(4) 6_565 .
O33 P6 O14 114.7(3) . .
O33 P6 O14 114.7(3) . 6_565
O14 P6 O14 107.0(3) . 6_565
O9 P7 O12 108.6(3) . .
O9 P7 O19 112.6(3) . .
O12 P7 O19 111.5(3) . .
O9 P7A O12 116.4(4) . .
O9 P7A O19 117.3(3) . .
O12 P7A O19 116.8(4) . .
O3 P8 O15 109.3(3) 2_757 .
O3 P8 O13 112.2(3) 2_757 .
O15 P8 O13 111.6(3) . .
O3 P8A O15 114.2(3) 2_757 .
O3 P8A O13 115.5(4) 2_757 .
O15 P8A O13 115.0(3) . .
O22 P9 O22 100.0(3) . 6_565
O22 P9 O21 102.1(2) . .
O22 P9 O21 102.1(2) 6_565 .
O22 P9 O28 114.2(2) . .
O22 P9 O28 114.2(2) 6_565 .
O21 P9 O28 121.2(3) . .
O21 P9A O22 100.2(3) . .
O21 P9A O22 100.2(2) . 6_565
O22 P9A O22 96.6(3) . 6_565
O21 P9A O30 124.9(3) . .
O22 P9A O30 115.1(2) . .
O22 P9A O30 115.1(2) 6_565 .
O16 P10A O16 97.9(3) 6_565 .
O16 P10A O8 101.94(19) 6_565 .
O16 P10A O8 101.94(19) . .
O16 P10A O32 115.0(2) 6_565 .
O16 P10A O32 115.0(2) . .
O8 P10A O32 121.6(4) . .
O16 P10 O16 97.2(3) 6_565 .
O16 P10 O8 101.3(2) 6_565 .
O16 P10 O8 101.3(2) . .
O16 P10 O31 115.5(2) 6_565 .
O16 P10 O31 115.5(2) . .
O8 P10 O31 122.1(3) . .
Mo3 O1 Mo1 83.49(11) . .
Mo3 O1 Co2 133.1(2) . .
Mo1 O1 Co2 140.7(2) . .
Mo3 O2 Mo1 83.15(11) . .
Mo3 O2 Co5 132.6(2) . .
Mo1 O2 Co5 140.8(2) . .
P8A O3 P8 31.70(18) 2_757 2_757
P8A O3 Mo1 139.7(3) 2_757 .
P8 O3 Mo1 142.5(3) 2_757 .
Mo4 O4 Mo2 83.71(16) . .
Mo4 O4 Co3 133.50(18) . .
Mo2 O4 Co3 140.35(15) . .
Mo4 O5 Mo2 83.69(16) . .
Mo4 O5 Co4 133.24(18) . .
Mo2 O5 Co4 139.62(16) . .
P3 O6 Mo4 136.8(2) . .
P5 O7 Mo4 135.2(2) . .
P10A O8 P10 55.0(2) . .
P10A O8 Mo3 113.44(9) . .
P10 O8 Mo3 112.98(10) . .
P10A O8 Mo3 113.44(9) . 6_565
P10 O8 Mo3 112.98(10) . 6_565
Mo3 O8 Mo3 127.2(2) . 6_565
P7A O9 P7 29.1(2) . .
P7A O9 Mo2 142.8(3) . .
P7 O9 Mo2 142.8(2) . .
P2 O10 Mo3 135.8(3) . .
P1 O11 Mo3 136.2(3) . .
P7A O12 P7 28.4(2) . .
P7A O12 Mo1 139.8(3) . .
P7 O12 Mo1 143.6(3) . .
P8A O13 P8 30.20(18) . .
P8A O13 Co2 123.1(2) . 2_757
P8 O13 Co2 131.4(2) . 2_757
P8A O13 Co4 122.6(3) . .
P8 O13 Co4 130.7(3) . .
Co2 O13 Co4 97.65(16) 2_757 .
P6 O14 Co3 122.4(2) . .
P6 O14 Co5 120.7(2) . .
Co3 O14 Co5 101.50(17) . .
P8A O15 P8 31.5(2) . .
P8A O15 Mo2 140.3(3) . .
P8 O15 Mo2 143.9(2) . .
P10A O16 P10 55.25(16) . .
P10A O16 Mo1 121.1(2) . .
P10 O16 Mo1 120.3(2) . .
P5 O17 Co3 124.36(17) . .
P5 O17 Co3 124.36(17) . 6_565
Co3 O17 Co3 103.79(17) . 6_565
P7A O19 P7 27.7(2) . .
P7A O19 Co5 124.6(2) . .
P7 O19 Co5 132.7(2) . .
P7A O19 Co3 123.2(3) . .
P7 O19 Co3 129.7(2) . .
Co5 O19 Co3 97.28(16) . .
P9 O21 P9A 55.5(2) . .
P9 O21 Mo4 113.76(14) . .
P9A O21 Mo4 112.81(13) . .
P9 O21 Mo4 113.76(14) . 6_565
P9A O21 Mo4 112.81(13) . 6_565
Mo4 O21 Mo4 126.90(16) . 6_565
P9 O22 P9A 55.1(2) . .
P9 O22 Mo2 122.13(19) . .
P9A O22 Mo2 120.2(2) . .
P3 O23 Co4 123.8(2) . .
P3 O23 Co4 123.8(2) . 6_565
Co4 O23 Co4 100.90(18) . 6_565
P1 O24 Co2 123.22(14) . 6_565
P1 O24 Co2 123.22(14) . .
Co2 O24 Co2 100.4(3) 6_565 .
P2 O27 Co5 122.94(13) . .
P2 O27 Co5 122.94(13) . 6_565
Co5 O27 Co5 104.5(3) . 6_565
P9 O28 Co4 111.0(2) . 6_565
P9 O28 Co4 111.0(2) . .
Co4 O28 Co4 97.0(2) 6_565 .
P4 O29 Co4 121.2(3) . 2_757
P4 O29 Co2 122.1(3) . .
Co4 O29 Co2 100.69(16) 2_757 .
P9A O30 Co3 110.8(2) . .
P9A O30 Co3 110.8(2) . 6_565
Co3 O30 Co3 95.75(19) . 6_565
P10 O31 Co2 113.1(2) . .
P10 O31 Co2 113.1(2) . 6_565
Co2 O31 Co2 94.9(2) . 6_565
P10A O32 Co5 112.7(3) . .
P10A O32 Co5 112.7(3) . 6_565
Co5 O32 Co5 96.2(3) . 6_565
C1 N1 C5 114.4(6) . .
C1 N1 Co2 119.5(4) . .
C5 N1 Co2 125.3(5) . .
C10 N2 C6 116.5(8) . .
C10 N2 Co3 121.9(7) . .
C6 N2 Co3 121.3(5) . .
C11 N3 C15 112.5(8) . .
C11 N3 Co4 122.3(6) . .
C15 N3 Co4 121.1(5) . .
C1A N1A C3A 103.1(5) . .
C1A N1A C1B 58.69(15) . .
C3A N1A C1B 55.4(4) . .
C1A N1A C5B 55.5(3) . .
C3A N1A C5B 103.4(4) . .
C1B N1A C5B 100.18(9) . .
C1A N1A Co5 125.8(2) . .
C3A N1A Co5 124.5(5) . .
C1B N1A Co5 128.63(9) . .
C5B N1A Co5 124.41(7) . .
N1A C1A C2A 108.8(3) . .
N1A C1A H1AA 125.6 . .
C2A C1A H1AA 125.6 . .
C1A C2A N2A 114.6(4) . .
N1A C3A N2A 111.9(6) . .
N1A C3A H3AA 124.0 . .
N2A C3A H3AA 124.1 . .
C2A N2A C3A 94.4(5) . .
C3B C2B C1B 100.12(9) . .
N1A C5B C4B 124.48(12) . .
N1A C5B H5BA 117.8 . .
C4B C5B H5BA 117.8 . .
C5B C4B C3B 114.72(12) . .
C5B C4B H4BA 122.6 . .
C3B C4B H4BA 122.6 . .
C2B C3B C4B 124.62(15) . .
C2B C3B H3BA 117.7 . .
C4B C3B H3BA 117.7 . .
N1A C1B C2B 136.56(15) . .
N1A C1B H1BA 111.7 . .
C2B C1B H1BA 111.7 . .
N1 C1 C2 122.7(7) . .
N1 C1 H1A 118.7 . .
C2 C1 H1A 118.7 . .
C1 C2 C3 116.6(9) . .
C1 C2 H2A 121.7 . .
C3 C2 H2A 121.7 . .
C4 C3 C2 120.7(9) . .
C4 C3 H3A 119.6 . .
C2 C3 H3A 119.6 . .
C3 C4 C5 120.6(8) . .
C3 C4 H4A 119.7 . .
C5 C4 H4A 119.7 . .
C4 C5 N1 125.0(8) . .
C4 C5 H5A 117.5 . .
N1 C5 H5A 117.5 . .
N2 C6 C7 125.8(8) . .
N2 C6 H6A 117.1 . .
C7 C6 H6A 117.1 . .
C8 C7 C6 117.3(9) . .
C8 C7 H7A 121.4 . .
C6 C7 H7A 121.4 . .
C7 C8 C9 122.5(9) . .
C7 C8 H8A 118.8 . .
C9 C8 H8A 118.8 . .
C8 C9 C10 117.6(10) . .
C8 C9 H9A 121.2 . .
C10 C9 H9A 121.2 . .
N2 C10 C9 120.3(10) . .
N2 C10 H10A 119.9 . .
C9 C10 H10A 119.9 . .
N3 C11 C12 119.8(10) . .
N3 C11 H11A 120.1 . .
C12 C11 H11A 120.1 . .
C13 C12 C11 122.7(10) . .
C13 C12 H12A 118.7 . .
C11 C12 H12A 118.7 . .
C14 C13 C12 115.6(9) . .
C14 C13 H13A 122.2 . .
C12 C13 H13A 122.2 . .
C13 C14 C15 116.1(9) . .
C13 C14 H14A 122.0 . .
C15 C14 H14A 122.0 . .
N3 C15 C14 128.9(9) . .
N3 C15 H15A 115.5 . .
C14 C15 H15A 115.5 . .
O1W O1W O5WA 69.2(18) 2_655 .
O2WB O2W O2W 128.1(5) . 6
O2WB O2W Co1 69.5(4) . .
O2W O2W Co1 65.5(3) 6 .
O1W O5W O5WA 65(7) 2_655 .
O1W O5WA O1W 42(4) 2_655 .
O1W O5WA O5W 20.8(18) 2_655 .
O1W O5WA O5W 20.8(18) . .
O2WA O2WA Co1 67.9(3) 6 .
O2W O2WB Co1 70.6(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O20 1.692(4) .
Mo1 O1 1.965(3) .
Mo1 O2 1.968(4) .
Mo1 O3 2.087(4) .
Mo1 O12 2.092(4) .
Mo1 O16 2.206(4) .
Mo1 Mo3 2.6016(8) .
Mo2 O26 1.677(4) .
Mo2 O4 1.963(4) .
Mo2 O5 1.966(4) .
Mo2 O15 2.081(4) .
Mo2 O9 2.094(4) .
Mo2 O22 2.173(4) .
Mo2 Mo4 2.6077(6) .
Mo3 O25 1.680(4) .
Mo3 O1 1.942(4) .
Mo3 O2 1.953(3) .
Mo3 O10 2.054(4) .
Mo3 O11 2.057(4) .
Mo3 O8 2.454(2) .
Mo4 O18 1.670(4) .
Mo4 O5 1.943(4) .
Mo4 O4 1.946(3) .
Mo4 O6 2.037(4) .
Mo4 O7 2.047(4) .
Mo4 O21 2.4650(18) .
Co1 O2WB 1.997(8) .
Co1 O2WB 1.997(8) 2_655
Co1 O2WB 1.997(8) 6
Co1 O2WB 1.997(8) 5_655
Co1 O2W 2.011(7) .
Co1 O2W 2.011(7) 6
Co1 O2W 2.011(7) 5_655
Co1 O2W 2.011(7) 2_655
Co1 O2WA 2.027(7) 6
Co1 O2WA 2.027(7) .
Co1 O2WA 2.027(7) 2_655
Co1 O2WA 2.027(7) 5_655
Co2 O1 2.045(3) .
Co2 O29 2.107(3) .
Co2 N1 2.131(6) .
Co2 O13 2.140(4) 2_757
Co2 O24 2.155(4) .
Co2 O31 2.248(4) .
Co3 O4 2.037(4) .
Co3 O14 2.072(4) .
Co3 N2 2.121(5) .
Co3 O17 2.134(3) .
Co3 O19 2.152(3) .
Co3 O30 2.264(3) .
Co4 O5 2.039(4) .
Co4 O29 2.077(5) 2_757
Co4 N3 2.107(5) .
Co4 O13 2.141(3) .
Co4 O23 2.176(3) .
Co4 O28 2.240(3) .
Co5 O2 2.038(3) .
Co5 O14 2.098(3) .
Co5 N1A 2.1441(14) .
Co5 O19 2.150(4) .
Co5 O27 2.154(4) .
Co5 O32 2.288(5) .
P1 O39 1.487(9) .
P1 O11 1.511(4) 6_565
P1 O11 1.511(4) .
P1 O24 1.526(6) .
P2 O37 1.488(10) .
P2 O10 1.527(4) .
P2 O10 1.527(4) 6_565
P2 O27 1.540(6) .
P3 O23 1.506(6) .
P3 O36 1.511(10) .
P3 O6 1.543(5) .
P3 O6 1.543(5) 6_565
P4 O35 1.478(9) .
P4 O35A 1.482(11) .
P4 O29 1.527(5) .
P4 O29 1.527(5) 6_565
P5 O17 1.516(5) .
P5 O38 1.531(10) .
P5 O7 1.549(5) 6_565
P5 O7 1.549(5) .
P6 O33 1.412(7) .
P6 O14 1.563(4) .
P6 O14 1.563(4) 6_565
P7 O9 1.487(6) .
P7 O12 1.524(3) .
P7 O19 1.540(5) .
P7A O9 1.426(6) .
P7A O12 1.452(5) .
P7A O19 1.522(5) .
P8 O3 1.501(4) 2_757
P8 O15 1.509(5) .
P8 O13 1.560(4) .
P8A O3 1.458(5) 2_757
P8A O15 1.464(6) .
P8A O13 1.546(5) .
P9 O22 1.580(4) .
P9 O22 1.580(4) 6_565
P9 O21 1.590(6) .
P9 O28 1.674(8) .
P9A O21 1.593(5) .
P9A O22 1.621(4) .
P9A O22 1.621(4) 6_565
P9A O30 1.633(7) .
P10A O16 1.582(4) 6_565
P10A O16 1.582(4) .
P10A O8 1.591(5) .
P10A O32 1.604(5) .
P10 O16 1.591(4) 6_565
P10 O16 1.591(4) .
P10 O8 1.597(5) .
P10 O31 1.612(5) .
O3 P8A 1.458(5) 2_757
O3 P8 1.501(4) 2_757
O8 Mo3 2.454(2) 6_565
O13 Co2 2.140(4) 2_757
O17 Co3 2.134(3) 6_565
O21 Mo4 2.4650(18) 6_565
O23 Co4 2.176(3) 6_565
O24 Co2 2.155(4) 6_565
O27 Co5 2.154(4) 6_565
O28 Co4 2.240(3) 6_565
O29 Co4 2.077(5) 2_757
O30 Co3 2.264(3) 6_565
O31 Co2 2.248(4) 6_565
O32 Co5 2.288(5) 6_565
N1 C1 1.338(9) .
N1 C5 1.345(8) .
N2 C10 1.294(13) .
N2 C6 1.329(10) .
N3 C11 1.310(10) .
N3 C15 1.325(9) .
N1A C1A 1.350(2) .
N1A C3A 1.351(3) .
N1A C1B 1.3700(9) .
N1A C5B 1.3700(9) .
C1A C2A 1.351(3) .
C1A H1AA 0.9300 .
C2A N2A 1.354(3) .
C3A N2A 1.501(11) .
C3A H3AA 0.9300 .
C2B C3B 1.3700(9) .
C2B C1B 1.3702(9) .
C5B C4B 1.3701(9) .
C5B H5BA 0.9300 .
C4B C3B 1.3701(9) .
C4B H4BA 0.9300 .
C3B H3BA 0.9300 .
C1B H1BA 0.9300 .
C1 C2 1.390(11) .
C1 H1A 0.9300 .
C2 C3 1.396(12) .
C2 H2A 0.9300 .
C3 C4 1.253(13) .
C3 H3A 0.9300 .
C4 C5 1.332(11) .
C4 H4A 0.9300 .
C5 H5A 0.9300 .
C6 C7 1.347(11) .
C6 H6A 0.9300 .
C7 C8 1.303(14) .
C7 H7A 0.9300 .
C8 C9 1.311(14) .
C8 H8A 0.9300 .
C9 C10 1.463(15) .
C9 H9A 0.9300 .
C10 H10A 0.9300 .
C11 C12 1.387(11) .
C11 H11A 0.9300 .
C12 C13 1.357(12) .
C12 H12A 0.9300 .
C13 C14 1.304(10) .
C13 H13A 0.9300 .
C14 C15 1.356(11) .
C14 H14A 0.9300 .
C15 H15A 0.9300 .
O1W O1W 0.83(7) 2_655
O1W O5WA 1.17(5) .
O2W O2WB 1.369(12) .
O2W O2W 1.67(2) 6
O5W O1W 0.46(4) 2_655
O5W O5WA 1.29(5) .
O5WA O1W 1.17(5) 2_655
O2WA O2WA 1.52(2) 6
